### Heat Transfer and Fluid Flow during Electron Beam Welding of 304L

Heat Transfer and Fluid Flow during Electron
Beam Welding of 304L Stainless Steel Alloy
Models were used to calculate the three-dimensional temperature field and fluid
velocities for electron beam welding of 304L stainless steel
BY R. RAI, T. A. PALMER, J. W. ELMER, AND T. DEBROY
ABSTRACT
m
g
z
o
J]
m
m
0)
>
O
A numerical model for three-dimensional heat transfer and fluid flow in
keyhole mode electron beam welding
was developed and applied to 304L
stainless steel welds made at different
power density distributions achieved
by varying the focal spot radius at a
fixed input power. The model first calculates keyhole geometry based on energy balance on keyhole walls and
then solves the three-dimensional
temperature field and fluid velocities
in the workpiece. Since the energy balance and, consequently, the keyhole
penetration are affected by the keyhole wall temperatures, the variation
of the keyhole wall temperature with
depth has been considered. A modified turbulence model based on
Prandtl's mixing length hypothesis was
used to calculate the spatially variable
effective values of thermal conductivity and viscosity to account for enhanced heat and mass transfer due to
turbulence in the weld pool. Unlike
models available in literature, the
model proposed in this work considers
the physical processes like variations
of keyhole wall temperatures with
depth and the resulting influence on
calculation of keyhole depth and fluid
velocities along the keyhole wall, and
three-dimensional heat and mass
transport. Thus, the model can be applied to materials with a range of thermophysical properties. The model was
used to study the fluid flow patterns in
the weld pool and their effects on the
calculated weld geometry. The calculated weld dimensions agreed reasonably well with the measured values.
Peclet number calculation showed
that convective heat transfer was very
R. RAI, T.A. PALMER, and T. DEBROY are with
Department ofMaterials Science and Engineering,
The Pennsylvania State University, University Park,
Pa. J. W. ELMER is with Lawrence Livermore National Laboratory, Livermore, Calif.
MARCH 2009, VOL. 88
significant. The influence of convection was illustrated by comparing the
calculated weld pool geometries in
the presence and absence of convection. The vapor pressures and wall
temperatures in the keyhole increased with increase in the peak
power density.
Introduction
High-energy-density electron beams
are often used to join a wide range of materials with an equally wide range of thicknesses for applications where a high aspect
ratio (depth/width) and narrow heataffected zone are needed. Due to the very
high intensity of electron beams, the workpiece material undergoes strong localized
evaporation, resulting in the formation of
a narrow and deep vapor cavity or "keyhole" (Refs. 1, 2). A pressure gradient
forms along the keyhole depth because of
the flow of metal vapor resulting in a variation in the equilibrium temperatures of
the keyhole walls with weld depth. Temperatures at the top and the bottom of the
keyhole can differ by several hundred degrees (Ref. 3), which results in the flow of
liquid metal in the vertical direction under
the influence of the surface-tension gradient along the keyhole walls.
While many numerical models for heat
transfer and fluid flow have been developed for keyhole mode laser welding
(Refs. 4—23), comprehensive heat transfer
r
KEYWORDS
Electron Beam Welding
Keyhole
Heat Transfer
Fluid Flow
Stainless Steel
Weld Process Simulation
Three-Dimensional
Phenomenological Model
and fluid flow models for electron beam
welding are not available in the literature.
Klemens (Ref. 7) performed pressure balance at the keyhole walls to calculate the
(Ref. 8) proposed a 3-D heat conduction
model for the calculation of temperature
profiles in the workpiece. Kaplan (Ref. 12)
and Zhao (Ref. 19) calculated the asymmetric keyhole profile at high welding
speeds by considering energy balance at
the keyhole walls. Sudnik et al. (Ref. 13)
approximated the 3-D fluid flow in the
weld pool by 2-D flows in horizontal and
vertical planes. Ki et al. (Refs. 17,18) calculated the transient evolution of the keyhole and the weld pool during laser welding using the level set method to track the
liquid-vapor interface. Rai et al. (Refs.
20-23) calculated the asymmetric keyhole
profile through energy balance at keyhole
walls considering multiple reflections of
the laser beam within the keyhole, and the
3-D heat transfer and fluid flow in the
weld pool. Elmer et al. (Ref. 24) proposed
three heat conduction models for electron
beam welding based on distributed, point,
or line heat sources, depending on the
power densities and compared calculated
and measured weld geometries. Wei and
Giedt (Ref. 25) proposed a twodimensional heat transfer and fluid flow
model and computed the free surface temperature, liquid layer thickness, and tangential free surface fluid velocities assuming the surface tension gradient to be the
main driving force for the fluid flow. Wei
and Chow (Ref. 26) studied the effect of
beam focusing and alloying elements on
the shape of the electron beam keyhole.
Assuming the vapor cavity to be a paraboloid of revolution, Wei and Shian (Ref. 27)
calculated penetration depth and surface
temperatures using an analytical threedimensional heat conduction model.
Here we propose a three-dimensional
phenomenological model for heat transfer
and fluid flow in electron beam welding
that considers keyhole formation and the
variation of keyhole wall temperature as a
function of depth. A very important parameter in the electron beam welding
A
A3
-ill
•0,1
0.0
3.0
0.1
X (uim)
Fig. 1 — Beam shape for 0.17-mm beam radius
produced at sharp focus settings for 1000-W power
at a work distance of 229 mm.
process is the power density distribution.
In this work, the model was applied to
welds made on 304L stainless steel with
fixed input power and welding speed but
different power density distributions. The
power density distribution was varied by
changing the work distance and then refocusing the electron beam to a sharp spot
on the workpiece surface. The increase in
the focal spot diameter with increasing
work distance also affects the geometry of
the weld pool shape (Ref. 28). The calculated and the experimental weld geometries were compared for each case and the
effect of variation of power density distribution on the weld geometry was investigated. The resulting fluid flow circulation
patterns in the 304L stainless steel electron beam weld pools were studied. The
electron beam welds observed in this study
was explained in terms of the fluid flow
and resulting convective heat transfer.
Experiments
Autogenous electron beam welds were
made on 9.5-mm-thick 304L stainless steel
samples with a power of 1000 W (100 kV,
10 mA) and a welding speed of 17 mm/s.
4.0
5.0
X, mm
6.0
2.0
1.0
%
3.0
4.0
5.0
6.0
X, mm
Fig. 2 — Fluid flow pattern in electron beam weld for focal spot radius of the following: A — 0.13 mm;
B — 0.28 mm. Labels 1, 2, and 3 represent 1697, 1900, and 2200 K, respectively,
The stainless steel workpiece had a composition of 18.2%Cr, 8.16%Ni, 1.71%Mn,
0.02%C, 0.082%N, 0.47%Mo, 0.44%Si,
0.14%Co, 0.35%Cu, 0.0004%S, 0.03%P,
and balance Fe. Six welds were made using
a sharply focused beam at different work
distances (Table 1). The resulting weld
pool cross sections were polished and
etched with electrolytic oxalic acid solution to provide the outline of the fusion
zone boundary. Image Pro, Version 4.1
was then used to measure the weld dimensions (Ref. 28).
The sharp focus condition was determined by using an enhanced modified
Faraday cup (EMFC) device to ensure a
more consistent and quantified beam
focus than is manually possible (Ref. 28).
The EMFC device samples the electron
beam through 17 linear slits placed radially around a tungsten slit disk and converts them into voltage drops across the
known resistor. A computer-assisted tomographic (CT) imaging algorithm is then
used to reconstruct the power density distribution of the beam using the data from
the 17 linear slits. From the reconstructed
beam, the peak power density, full width
of the beam at half of its peak intensity
(FWHM), and the full width of the beam
at 1/e2 of the peak intensity (FWe2) are
measured. The beam radius was taken to
be Vi of the FWe2 value measured by the
EMFC. Figure 1 shows the beam shape for
the case of a 0.17-mm focal spot radius,
from EB welding machine model number
SN/175 manufactured by Hamilton Standard at a 229-mm work distance (Ref. 28).
Since the beam has an elliptical shape, the <
effective value of the beam radius was LU
taken as the radius of a circle with an area
equal to the actual beam spot (Ref. 28). LU
The beam shape and radius may vary with
0C
distance from the focal plane, which can
affect the weld geometry. However, due to
a lack of data on the divergence of the
beam near the focal plane, its effect has
been neglected in this work.
o
if)
O
Mathematical Model
LU
Calculation of Keyhole Profile
Quasi-steady state and flat top surface
outside the keyhole region are assumed.
The fluctuations of the keyhole shape and
size have been neglected. Energy balance
is performed on the liquid-vapor interface
to calculate the keyhole geometry using a
model that is available in literature (Refs.
Table 1 — Experimental and Calculated Weld Dimensions for Welds Made at 1000-W Input Power and 17 mm/s Welding Speed Using Electron
Beam Welding Machine S/N 175
%
%
WD
mm
Rf
mm
PPD
kW/mm2
dm
mm
dc
mm
m
mm
w
c
mm
error
MA
mm2
AR
error
127
184
229
305
381
457
0.131
0.166
0.173
0.207
0.243
0.279
34.9
21.6
20.0
14.1
10.2
7.79
4.46
4.21
3.97
3.69
3.39
2.96
4.20
3.87
3.80
3.56
3.33
2.97
-6.19
-8.79
-4.47
-3.65
-1.80
0.34
1.27
1.29
1.48
1.48
1.55
1.71
1.38
1.52
1.58
1.68
1.76
1.90
7.97
15.13
6.33
11.90
11.93
10.00
2.40
2.55
2.63
2.58
2.56
2.62
3.52
3.27
2.65
2.49
2.19
1.73
w
WD; work-distance, Rj: radius of focal spot; PPD: peak power density; d; depth; w: width; subscripts m and c stand for measured and calculated; MA: melted cross-sectional
area; AR: aspect ratio.
WELDING JOURNAL
5
9.0
E 8.0
E
N
7.0
100 mm/s
6.0
2.0
-1.0
A
o.o
1.0
'-1.0
Y, mm
B
o.o
i.o
Y, mm
' :i.o
C
o.o
3.0
i.o
4.0
5.0
X , mm
6.0
Y, mm
7.0100 mm/s
6.0
2.0
-1.0
D
m
o
m
0)
m
>
33
O
0.0
-1.0
1.0
Y, mm
E
0.0
Y, mm
1.0
1.0
F
0.0
Y, mm
N
7.0100 mm/s
2.0
Physical Property
Solidus temperature, (K) [Refs. 23, 48]
Liquidus temperature, (K) [Refs. 23, 48]
Density of liquid (kg/m3) [Ref. 23]
Specific heat of solid, (J/kg K) [Ref. 23]
Specific heat of liquid, (J/kg K) [Ref. 23]
Viscosity, (Pa-s) [Ref. 23]
Coefficient of thermal expansion, (1/K) [Ref. 23]
Temperature coefficient of surface tension, (N/m K) [Ref. 48]
Enthalpy of solid at melting point, (J/kg) [Refs. 23, 48]
Enthalpy of liquid at melting point, (J/kg) [Refs. 23, 48]
Emissivity
Heat transfer coefficient, W/m2-K
Plasma attenuation coefficient, (nr1)
Absorption coefficient
Values are estimated based on the data available in the reference.
MARCH 2009, VOL. 88
Value
1697
1727
7000
712
800
0.007
1.96 x 10-5
-0.43xl0-3
1.20 xlO6
1.26 xlO6
0.3
210
10
0.2
3.0
4.0
5.0
X , mm
6.0
(1)
where p is the density, g is the acceleration
due to gravity, Y(T) is the surface tension
at temperature T, and r(z) is the keyhole
radius at distance z from the top surface.
The decrease in r(z) with increasing depth
in the keyhole results in an increase in the
surface tension force. As a result, the
vapor pressure required to keep the keyhole open increases with depth. Thus, the
vapor pressure at various depths in the
keyhole can be calculated from the above
equation.
The temperature at the keyhole wall at
any depth can then be calculated from the
Table 2 — Data Used for Calculations
6.0
E 8.0E
6.0
p = pgz + Y(T)/r(z)
4.0
5.0
X , mm
9.0-
1.0
Fig. 3 — Fluid flow in the weld made with 0.28-mm beam radius in transverse planes at the following
locations behind the electron beam: A — 0.11 mm; B — 0.28 mm; C — 0.45 mm; D — 0.62 mm; E —
ft 78 mm; and F — 0.95 mm. Only the top 3.5 mm of the total plate thickness of 9.5 mm is shown.
12, 19-23). The temperature gradient in
the vertical direction is small compared to
that along any direction in the horizontal
plane. Therefore, the heat transfer takes
place mainly along horizontal planes.
However, the temperature gradient on the
keyhole walls along the vertical direction
is still sufficient to generate surface tension driven flow along the keyhole walls in
the vertical direction.
The keyhole is kept open by a balance
between the surface tension force ylr{z),
the hydrostatic force due to the liquid
head pgz, and the vapor pressure inside
the keyhole p through the following
relationship:
3.0
Fig. 4 — Fluid flow in the weld made with 0.28mm beam radius in longitudinal planes at the
following locations from the centerline: A — 0
mm; B — 0.28 mm; and C — 0.45 mm. Labels
1, 2, and 3 represent 1697,1900, and 2200 K, respectively. Only the top 3.5 mm of the total plate
thickness of 9.5 mm is shown.
equilibrium temperature vs. pressure relation for the alloy-vapor interface assuming
ideal solution behavior (Ref. 29). The keyhole geometry is iteratively calculated first
by assuming a constant temperature equal
to the normal boiling point of the alloy at
1 atmosphere on the keyhole walls. The
calculation of the energy balance at the
keyhole walls is described elsewhere
(Refs. 12,19-23). The wall temperature is
modified in subsequent iterations by first
calculating the vapor pressure required to
balance the surface tension and the hydrostatic force at the keyhole wall. Using
this calculated vapor pressure, the wall
temperature is then determined through
equilibrium temperature vs. pressure relation, changing the keyhole depth and radius. Thus, the wall temperatures are corrected with each iteration, and the
calculations continue until the change in
keyhole depth with each additional iteration becomes less than 10^ mm, at which
point the calculations are assumed to con-
1 . U W wr—i
A
", WA
".--1
1 . _
4.0-
1
:T:T:t
^^^
E
E
•m
3.00)
Q
•
on
Measured
•
^^^
Calculated
— Linear (Measured) - - - • Linear (Calculated)
0. 13
0.18
0.23
0. 28
9 A
B
-1
- - - •
1.6r ~ " '
E
E
.
•
-
•
Measured
•
- - - • Linear (Calculated)
0. 13
f
8
0.8-
4-1
•o
:-
9
•
0.18
0.23
Calculated
7
Linear (Measured)
6
0
1
Y, mm
1
V
5^
-1
0.28
O
0
1
Y, mm
<
Fig. 5 —A — Variation of weld depth with spot radius; B — variation of weld width with spot radius.
verge. During calculation of the asymmetric keyhole geometry, all temperatures inside the keyhole were assigned the wall
temperature at that depth, for the identification of the keyhole. At each horizontal
xy plane, where x is the direction of welding, the keyhole boundary was identified
by both minimum and maximum x values
for any given}1 value.
The attenuation of the beam due to absorption and scattering, as it traverses a
unit distance in the plasma, is estimated by
using attenuation coefficients (Ref. 12).
The beam attenuation affects the amount
of electron beam energy incident on keyhole walls below the workpiece surface. It
is assumed that the energy loss due to
large angle backscattering of electrons by
the plasma in a deep, narrow keyhole is
small (Ref. 30). Consequently, a small
value of attenuation coefficient has been
assumed here for the attenuation of the
electron beam. With a plasma attenuation
coefficient value of 10/m used for electron
beam plasma here, 99% and 96% of the
electron beam passes through lengths of 1
and 4 mm, respectively, through the
plasma. Table 2 lists the values of material
properties and process parameters used
for the calculations. Thermal conductivity
values for the solid phase were temperature dependent and the thermal conductivity data were available up to a temperature of 1273 K. Approximate thermal
conductivity values above this temperature were estimated based on linear extrapolation of the experimental data for
304L stainless steel (Ref. 31). Thermal
conductivity for liquid was calculated
based on the Wiedemann-Franz relation,
which states that the ratio of thermal conductivity to the product of temperature
and electrical conductivity is a constant
(Ref. 32). The electrical conductivity of
liquid stainless steel was taken as the electrical conductivity of liquid iron at its theoretical melting point, which was close to
the value obtained by extrapolating the
data for electrical resistivity of 18Cr-8Ni
steel between 300 and 1273 K to the liquidus temperature (Ref. 29).
Heat Transfer and Fluid Flow in the Weld
Pool
After calculating the keyhole profile,
the fluid flow and heat transfer in the weld
pool are modeled by solving the equations
of conservation of mass, momentum, and
energy in three dimensions. The liquid
Kg. 6 — Comparison of experimental and calculated weld geometries for focal spot radii: A —
0.131 mm; B —0.173 mm; C —0.207 mm; D—
0.243 mm; E — 0.279 mm. Input power: 1000 W.
Welding speed: 17 mmls.
LU
TTT
\Ji
III
ff
•"
o
metal flow in the weld pool can be repre- ~~
sented by the following momentum con- ^J
servation equation (Refs. 33, 34):
^J
m
du
dlu.u.
du
dt
etc.
ar.
(2)
where p is the density, t is the time, J:;- is the
distance along the ;'"' (i = 1, 2, and 3) orthogonal direction, u; is the velocity component along the j direction, |i is the effective viscosity, and S: is the source term
for the /* momentum equation and is
given as
{
dp
S.=
c
|
9
doc.
dx.
J
'
U)
V
I1
v
du?
1
dx.
1J
2^
u +
1
*sAT-T*t)
J
du.
pi J
'
dx
(3)
where/? represents pressure, f/is the weldWELDING JOURNAL
A0.28mm
|o.6-
•0.13 mm |
- V II
9
•
•
3 0,4-
•
5 0.2-
E
E
>
N
0.0
0.5
1.0
1.5
2.0 2.5
z, mm
3.0
3.5
8
Fig. 7— Variation of vapor pressure in the keyhole
with depth for radius of 0.13 and 0.28 mm. z = 0 at
the surface of the workpiece.
A
,"
3000 -
<D
^ 2800 -
.-•l
V
E
E
• ••"
N
E
0)
O. 2600 -
E
u
^
8
6
5
0.5
1.0
1.5
2.0
2.5
3.0
3.5
4.0
z, mm
^^ Fig. 8 — Variation of keyhole wall temperature with
^0 depth for radius of 0.13 and 0.28 mm. z = Oat the
^" surface of the workpiece.
Jx
1
5_
0
1
Y, mm
c
w
^
y
rVY
1
Y
0
1
Y, mm
B
9 -
\ i
i i
8 -
I)
:
5_
1
o
A 3-D Cartesian coordinate system is
used in the calculation, and only half of the
workpiece is considered since the weld is
The boundary conditions are discussed as
follows.
E
E
7
N
7
.A4*
0.0
-
tions were solved for the complete workpiece. For the region inside the keyhole,
the coefficients and source terms in the
discretized algebraic equations were adjusted to obtain zero fluid velocities and
temperature equal to the wall temperature at that depth. The methodology for
the implementation of known values of
variables in any specified location of the
solution domain is well documented in the
literature (Ref. 34).
Boundary Conditions
9
^
i
6
:
•0 13 mm I
7
N
6
40
II II
8
E
E
7
5_
4 0 28 mm
A\:
9 -
;
;
1
6
0
Y, mm
Top Surface
-
Y, mm
D
Fig. 9 — Weld pool cross sections for focal spot
radius of 0.13 mm: A — With convection and B
— without convection; and 0.28 mm: C — with
convection and D — without convection. Input
power: 1000 W, welding speed: 17 mm/s.
Outside the region of vapor cavity, the
weld top surface is assumed to be flat. The
velocity boundary conditions are given as
(Refs. 40-43)
du _
dz
>
33
o
dT dx
dy dT
— = /L
dz
dT dy
o
m
(/)
m
rfy_9r
L
ing velocity, (3 is the coefficient of volume
expansion, and TWis a reference temperature taken here as the solidus temperature. The third term represents the frictional dissipation in the mushy zone
according to the Carman-Kozeny equation for flow through a porous media
(Refs. 35, 36), where/^ is the liquid fraction, fi is a very small computational constant introduced to avoid division by zero,
and C is a constant accounting for the
mushy zone morphology (a value of 1.6 x
104 was used in the present study) (Ref.
36). The fourth term is the buoyancy
source term (Refs. 37-41). The last term
accounts for the relative motion between
the electron beam and the workpiece
(Ref. 37).
The following continuity equation is
solved in conjunction with the momentum
equation to obtain the pressure field.
heat of fusion. The liquid fraction/^ is assumed to vary linearly with temperature
for simplicity (Ref. 37):
T>T,
T-T„
T <T<T
T
L- S
r<r
where 7^ and Tg are the liquidus and
solidus temperatures, respectively. Thus,
the transport of thermal energy in the
weld workpiece can be expressed by the
following modified energy equation:
=0
(4)
In order to trace the weld pool liquid/solid interface, i.e., the phase change,
the total enthalpy H is represented by a
sum of sensible heat h and latent heat content AH, i.e., H = h + AH (Ref. 37). The
sensible heat 'h' is expressed as \\=\C„dT,
where C„ is the specific heat, and T is the
temperature. The latent heat content A/f
is given as AH=fj^L, where L is the latent
MARCH 2009, VOL. 88
(8)
where u, v, and w are the velocity components along the x, y, and z directions, respectively, and dy/dT is the temperature
coefficient of surface tension. As shown in
this equation, the u and v velocities are determined from the Marangoni effect
(Refs. 40-43). The w velocity is equal to
zero since the outward flow at the top surface is assumed to be negligible.
The heat flux at the top surface is given
f[x2+y2]
92
tap
2
TVb
-oel TA-TA\-h{T-T\
_k_dh_ + S
„
dx. C dx
V P '
p—+P^—'-=—
dt
rk.
(5)
T
w=0
cbc.
(6)
Mu.AH]
dt
rk.
i
dAH
-pU^-pU
(k
cte
(9)
;=1
where k is the thermal conductivity. The
source term S^ is due to the latent heat
content and is given as
dlAH)
-Th
J .
^^ V,l V,l
(7)
The heat transfer and fluid flow equa-
power distribution factor, Q is the total
power, r) is the absorption coefficient, o is
the Stefan-Boltzmann constant, e is the
emissivity, hc is the heat transfer coefficient, hv i is the heat of evaporation for the
i"1 element, Jv;- is the evaporation flux for
the i"1 element calculated using the Langmuir equation (Ref. 1), and Ta is the ambient temperature. In Equation 9, the first
term on the right-hand side is the heat
input from the Gaussian heat source. The
second, third, and fourth terms represent
the heat loss by radiation, convection, and
vaporization, respectively.
Symmetric Plane
The boundary conditions are defined
as zero flux across the symmetric surface,
i.e., the vertical plane defined by the welding direction, as
(10)
dy
dy
—=0
dy
(11)
Keyhole Surface
h = h„
(12)
where hw is the sensible heat of the material at the local wall temperature. The velocity component perpendicular to the
keyhole surface is assigned zero to represent no mass flux due to convection. Along
the keyhole walls, the temperature gradient in the vertical direction results in the
surface tension gradient. As a result,
Marangoni convection currents are
formed in the vertical direction along the
surface of the keyhole. The w-velocity
boundary condition along the keyhole
walls is therefore given as
dn
L
where |a,f is the turbulent viscosity, lm is the
mixing length, and vf is the turbulence velocity. The mixing length at any location
within the weld pool is the distance traveled by an eddy before its decay and is
often taken as the distance from the nearest wall (Ref. 45). The extent of computed
turbulent kinetic energy was found to be
about 10% of the mean kinetic energy, in
a controlled numerical study of recirculating flows in a small square cavity (Ref. 46).
Yang and DebRoy (Ref. 47) computed
mean velocity and turbulent energy fields
during GMA welding of HSLA 100 steel
using a two equation k-e model. Their results also show that there is a 10% contribution of the turbulent kinetic energy to
the mean kinetic energy. The turbulent velocity vt can therefore be expressed as
,4lv
z
(15)
By coupling Equations 14 and 15, the
turbulent viscosity can be expressed as
\it = 0.3p/mv
(16)
The effective viscosity at a particular
point can be expressed as the sum of the
turbulent (|if) and laminar (|a^) viscosities,
i.e., [>. = \it + |i;. The corresponding local
turbulent thermal conductivities are calculated by using the turbulent Prandtl
number, which is defined in the following
relationship:
^c
Solid Surfaces
At all solid surfaces far away from the
heat source, a convective heat transfer
boundary condition is given and the velocities are set to be zero.
The presence of fluctuating velocities
during welding often enhances the rates of
transport of heat, mass, and momentum in
the weld pool. An appropriate turbulence
model that provides a systematic framework for calculating effective viscosity and
thermal conductivity (Refs. 41, 42) is used
to account for the fluctuating velocities.
The values of these properties vary with
the location in the weld pool and depend
on the local characteristics of the fluid
flow. In this work, a turbulence model
based on Prandtl's mixing length hypothesis is used to estimate the turbulent viscosity (Ref. 45)
^ = P1m
, vt
Pr--
' p
(17)
where kt is the turbulent thermal conductivity. For the calculations described here,
the turbulent thermal conductivity is calculated by assuming a Prandtl number of
0.9, based on previous modeling work
(Refs. 44, 46).
Calculation Methodology
Turbulence Model
(14)
Results and Discussion
Figure 2 shows the computed weld
geometry and the 3-D fluid flow within the
weld pool for the welds made with the
highest (0.28 mm) and the lowest (0.13
mm) beam radii at input power of 1000 W
and welding speed of 17 mm/s. The flow of
molten metal is driven by the surface tension gradient along the keyhole walls and <
on the top surface of the weld pool. A neg- LU
ative temperature coefficient of surface (/)
tension drives fluid flow at the top surface LU
from the high-temperature region near
0C
the keyhole to the low-temperature region
near the solid-liquid boundary, resulting
in enhanced heat transfer at the top
surface.
Within the keyhole, temperatures are
highest at the bottom and lowest near the
along the keyhole surface drives fluid flow LU
from the hot keyhole bottom to the top,
resulting in a fluid flow pattern in the weld
pool where hot fluid moves along the keyhole walls to the top, moving outward
from there, and finally coming back inward and down along the solid-liquid
boundary. A distinct nail-head shape results from this type of fluid flow pattern.
Figure 3 shows the fluid flow in transverse planes perpendicular to the welding
direction at selected distances from the
heat source. Plane 'a' is the closest to the
electron beam location (0.11 mm) and
plane 'f is the farthest behind the electron
beam (0.95 mm). The keyhole region,
which is characterized by the absence of
velocity vectors at the center of the weld
pool, is present only in Fig. 3A. Under the
the vapor-liquid interface, the fluid near
the keyhole wall moves from the bottom to
the top. The magnitude of fluid velocities
in the vertical direction is highest near the
vapor-liquid interface and decreases to
zero at the solid-liquid boundary. As the
o
O
(13)
dT dz
where n is the direction vector normal to
the keyhole surface.
5. Steps 2-4 are repeated until the variation of keyhole depth with further iteration becomes less than 10^ mm.
6. The keyhole geometry is mapped
onto a coarser mesh for 3-D heat transfer
and fluid flow calculations. Temperatures
are assigned on the keyhole wall from the
values calculated during keyhole geometry calculation based on equilibrium pressure-temperature relations for the alloy.
7. The momentum and energy balance
equations are solved keeping fixed temperatures on the keyhole wall, and assuming no mass flux across the wall boundary.
Convergence was assumed when residuals
of enthalpy and u, v, and w velocities are
less than 1%.
8. A turbulence model is used to update the viscosities and thermal conductivities in the liquid phase.
The calculation of heat transfer and
fluid flow in the workpiece was done in the
following steps:
1. The keyhole geometry is calculated
based on a heat balance model available in
the literature (Ref. 17) and boiling point
temperature at all locations on the keyhole wall.
2. The vapor pressure in the keyhole is
calculated at all depths through a force
balance between the vapor pressure, surface tension, and hydrostatic force.
3. Wall temperatures are calculated for
all depths from the equilibrium pressuretemperature relations for the given alloy.
4. Keyhole geometry is calculated assuming new values of wall temperatures at
different depths.
5
WELDING JOURNAL
m
g
z
o
m
m
(/)
>
33
o
distance of the transverse section from the
starts to come downward and the reversal
of the direction of fluid velocity from upward to downward happens at shorter distances from the top surface.
In the longitudinal sections shown in
Fig. 4, the fluid moves upward near the
heat source location and circulates backward near the top surface resulting in enhanced heat transfer toward the rear of
the weld pool and an elongated weld pool.
The circulation pattern is similar in all of
the longitudinal sections shown in Fig. 4
located at different distances from the
weld centerline.
As shown in Table 1, an increase in
work distance from 127 to 457 mm resulted in more than a twofold increase in
the beam focal spot radius (Rf). With a
larger focal spot radius, the beam is more
diffuse and the peak power density is
lower, decreasing from 34.9 kW/mm2 for
127-mm work distance (focal radius =
0.13 mm) to 7.79 kW/mm2 for 457-mm
work distance (focal radius = 0.28 mm)
(Ref. 28). As a result, the weld characteristics are likely to be strongly affected by
the variation in beam radius. Figure 5A, B
shows the variation of weld pool depth and
width at the top surface, respectively, with
the variation in the focal spot radius. The
calculated weld width and depth display
trends similar to the measured values.
With an increase in beam radius, the input
energy distribution is more diffuse and the
peak power density decreases, thus decreasing the weld penetration. However, a
larger focal spot radius increases melting
on the top surface, resulting in a wider
weld pool. Thus, the ratio of weld pool
depth to width decreases with increasing
beam radii, as shown in Table 1. The area
of calculated weld cross section is nearly
constant with variation in the beam radius.
Figure 6 shows the comparison of calculated and experimental weld cross sections for different focal spot radii. The
dashed lines show the calculated keyhole
profile. The calculated keyhole radius at
the top surface of the weld is closely related
to the electron beam radius. The calculated
weld cross sections are similar to the experimentally observed weld cross sections.
shape of the weld cross section is predicted
by calculations as well. Even though the
beam divergence may contribute to the
nail-head shape, this characteristic shape of
electron beam welds can also be explained
in terms of Marangoni convection.
The keyhole and weld geometry depends on the keyhole wall temperatures,
which in turn depend on the vapor pressure in the keyhole. Figure 7 shows the
variation of vapor pressure with depth for
beam radii of 0.13 and 0.28 mm. For the
welds shown in Fig. 6, the keyhole be-
MARCH 2009, VOL. 88
comes narrower and deeper as the beam
radius is decreased. The narrower keyhole for lower focal spot radius requires
a larger vapor pressure to balance the
surface tension force that tends to close
the keyhole. Therefore, vapor pressures
are higher for the higher peak power densities obtained with the smaller focal spot
radii. In accordance with higher vapor
pressures in the keyhole for the smaller
beam radius, equilibrium wall temperatures at the keyhole walls are higher for
the beam radius of 0.13 mm as compared
to the larger beam radius of 0.28 mm as
shown in Fig. 8. The higher keyhole wall
temperatures calculated for the smaller
focal spot radius are consistent with more
intense heating. The average temperature gradient in the perpendicular-towelding direction was always significantly
higher than that along the keyhole wall in
the vertical direction. For example, for
0.28 mm, the average temperature gradient in the weld pool at mid-height of the
keyhole in the horizontal direction was
about 26 times that in the vertical direction. Thus, the assumption that the temperature gradient in the vertical direction
is small compared to that in the horizontal plane is justified. Since the variation
of vapor pressure from the bottom to the
top of the keyhole results in less than a
15% variation in the wall temperature,
any errors in vapor pressure calculation
are likely to result in much smaller errors
in the computed wall temperatures.
The significance of convective heat
transfer relative to conductive heat transfer is given by the Peclet number,
Pe=pMCp(viV2)/&:,where p is the density, u
is the characteristic velocity, £„ is the specific heat, w is the weld pool width, and k
is the thermal conductivity. Using p =
7000 kg/m3, u = 0.1 m/s (the value of reference velocity vector in Fig. 2), Cp = 800
J/kg-K, w/2 = 8.0 x 10-4 m, andlc = 30
W/m-K, Pe = 14.9. Therefore, convective
heat transfer is very important for the
welding conditions studied here.
To further illustrate the significance of
convection on the weld pool geometry,
the temperature field in the workpiece
was calculated by considering only conductive heat transfer and ignoring fluid
flow. Figure 9A, C shows the calculated
weld pool cross sections for the case of
0.13- and 0.28-mm focal spot radius, respectively, with convection, and Fig. 9B,
D shows the corresponding weld cross
sections in the absence of any convection.
In the absence of convection, heat transfer is significantly reduced, which results
in much narrower weld pools. The calculated weld pool in absence of convection
also lacks the nail head shape usually observed in experiments because of the absence of enhanced outward heat transfer
at the top surface of the workpiece. The
differences in shape and size of the calculated weld pools in absence of and in
the presence of convection indicate the
significance of convective heat transfer
under the conditions considered.
Summary and Conclusions
The geometry of the keyhole formed
during electron beam welding was calculated through an energy balance at the
keyhole walls considering the variation of
vapor pressure and keyhole wall temperature with depth. A numerical heat transfer
and fluid flow model was used to calculate
the three-dimensional temperature field
and fluid velocities for electron beam
welding of 304L stainless steel. A turbulence model based on Prandtl's mixing
length hypothesis was used to estimate the
effective viscosities and thermal conductivities in the weld pool. The vapor pressure in the keyhole was calculated through
a force balance on the keyhole wall considering the surface tension force, the hydrostatic force, and the force due to vapor
pressure. The wall temperatures were calculated from equilibrium temperaturepressure relations for the alloy.
The calculated weld pool depth and
width were compared with experimentally observed values for a set of experiments where the power density distribution was varied by changing the focal spot
radius at a fixed input power. As the focal
spot size increased and the power distribution became progressively diffuse, the
penetration depth decreased and the
weld width increased proportionally in
order to maintain the total weld crosssectional area for the fixed input power.
Higher peak power density with the same
input power resulted in higher peak temperature and vapor pressure at the keyhole bottom. Fluid circulation in the weld
pool was studied for transverse sections
located at different distances from the
electron beam. Convective heat transfer
was very significant in determining the
weld geometry, as shown by Peclet number calculations. In the absence of convection, the calculated nail head shape of
the weld pool was not obtained. The reduced heat transfer near the top surface
in the absence of convection resulted in a
much narrower calculated weld pool, further illustrating the significance of convective heat transfer for the conditions of
welding considered.
Acknowledgment
The work was supported by a grant
from the U.S. Department of Energy, Office of Basic Energy Sciences, Division of
Materials Sciences, under grant number
DE-FGO2-01ER45900.
References
1. DebRoy, T, and David, S. A. 1995. Physical processes in fusion welding. Reviews of
Modem Physics 67: 85-112.
2. David, S. A., and DebRoy, T. 1992. Current issues and problems in welding science.
Science 257: 497-502.
3. Schauer, D. A., Giedt, W. H., and Shintaku, S. M. 1978. Electron beam welding cavity
temperature distributions in pure metals and alloys. Welding Journal 57(5): 127-s to 133-s.
4. Klein, T, Vicanek, M., Kroos, J., Decker,
I., and Simon, G. 1994. Oscillations of the keyhole in penetration laser beam welding. Journal
of Physics D: Applied Physics 27: 2023-2030.
5. Swift-Hook, D. E., and Gick, A. E. F.
1973. Penetration welding with lasers. Welding
Journal 52: 492-s to 499-s.
6. Andrews, J. G., and Atthey, D. R. 1976.
Hydrodynamic limit to penetration of a material by a high power beam. Journal of Physics D:
Applied Physics 9: 2181-2194.
I. Klemens, P. G. 1976. Heat balance and
flow conditions for electron beam and laser
welding. Journal of Applied Physics 47:
2165-2174.
8. Mazumder, J., and Steen, W. M. 1980.
Heat transfer model for cw laser material processing. Journal ofApplied Physics 51: 941-947.
9. Postacioglu, N., Kapadia, P., Davis, M.,
and Dowden J. 1987. Upwelling in the liquid region surrounding the keyhole in penetration
welding with a laser. Journal of Physics D: Applied Physics 20: 340-315.
10. Kroos, J., Gratzke, U., and Simon, G.
1993. Towards a self-consistent model of the keyhole in penetration laser beam welding. Journal
of Physics D: Applied Physics 26: 474 to 480.
II. Metzbower, E. A. 1993. Keyhole formation. Metallurgical Transactions B 24: 875-880.
12. Kaplan, A. 1994. A model of deep penetration laser welding based on calculation of
the keyhole profile. Journal of Physics D: Applied Physics 21: 1805-1814.
13. Sudnik, W., Radaj, D., and Erofeew, W.
1996. Computerized simulation of laser beam
welding, modelling and verification. Journal of
Physics D: Applied Physics 29: 2811-2817.
14. Matsunawa, A., and Semak, V 1997. The
simulation of front keyhole wall dynamics during laser welding. Journal of Physics D: Applied
Physics 30: 798-809.
15. Solana, P., and Ocana, J. L. 1997. A
mathematical model for penetration laser welding as a free-boundary problem. Journal of
Physics D: Applied Physics 30: 1300-1313.
16. Pastor, M., Zhao, H, Martukanitz, R. P.,
and DebRoy, T 1999. Porosity, underfill and
magnesium loss during continuous wave
Nd:YAG laser welding of thin plates of aluminum alloys 5182 and 5754. Welding Journal
78(6): 207-s to 216-s.
17. Ki, H, Mohanty, P. S., and Mazumder, J.
2002. Modeling of laser keyhole welding: Part I.
Mathematical modeling, numerical methodology, role of recoil pressure, multiple reflections,
and free-surface evolution. Metallurgical and
Materials Transactions A 33A: 1817 to 1830.
18. Ki, H, Mohanty, P. S., and Mazumder, J.
2002. Simulation of keyhole evolution, velocity,
temperature profile, and experimental veniication. Metallurgical and Materials Transactions A,
33A: 1831-1842.
19. Zhao, H, and DebRoy, T 2003. Macroporosity free aluminum alloy weldments
through numerical simulation of keyhole mode
laser welding. Journal of Applied Physics 93:
10089 to 10096.
20. Rai, R. and DebRoy, T 2006. Tailoring
weld geometry during keyhole mode laser welding using a genetic algorithm and a heat transfer model. Journal of Physics D: Applied Physics
39: 1257 to 66.
21. Rai, R., Roy, G G, and DebRoy, T
2007. A computationally efficient model of convective heat transfer and solidification characteristics during keyhole mode laser welding.
Journal of Applied Physics 101: article #054909.
22. Rai, R., Kelly, S. M., Martukanitz, R. P.,
and DebRoy, T 2008. A convective heat-transfer model for partial and full penetration keyhole mode laser welding of a structural steel.
Metallurgical and Materials Transactions A 39A
(1): 98 to 112.
23. Rai, R., Elmer, J. W, Palmer, T A., and
DebRoy, T 2007. Heat transfer and fluid flow
during keyhole mode laser welding of tantalum,
Ti-6AWV, 304L stainless steel and vanadium.
Journal of Physics D: Applied Physics 40: 5753 to
5766.
24. Elmer, J. W., Giedt, W. H, and Eagar, T
W. 1990. The transition from shallow to deep
penetration during electron-beam welding.
Welding Journal 69(5): 167-s to 176-s.
25. Wei, P. S., and Giedt, W. H. 1985. Surface
tension gradient-driven flow around an electron beam welding cavity. Welding Journal 64:
251-s to 259-s.
26. Wei, P. S., and Chow, Y. T 1992. Beam
focusing characteristics and alloying element
effect on high-intensity electron beam welding.
Metallurgical Transactions B 23B: 81 to 90.
27. Wei, P. S., Ho, C. ¥., Shian, M. D., and
Hu, C L. 1997. Three-dimensional analytical
temperature field and its application to solidification characteristics in high- or low-powerdensity beam welding. International Journal of
Heat and Mass Transfer 40: 2283-2292.
28. Elmer, J. W, and Teruya, A. T 1998. Fast
method for measuring power-density distribution of non-circular and irregular electron
beams. Science and Technology of Welding and
Joining 3(2): 51-58.
29. Brandes, E. A., and Brook, G B. 1992.
Smithells Metals Reference Book, 7th ed., Butterworth Heinemann, Mass.
30. Schiller, S., Heisig, U., and Panzer, S.
1982. Electron Beam Technology, John Wiley
and Sons, Berlin, Germany.
31. Kaye, G. W C, and Laby, T B. 1995. Tables of Physical and Chemical Constants, Longman, London, UK.
32. Lancaster, J. F 1986. The Physics of
Welding, Pergamon Press, Oxford, UK.
33. Bird, R. B., Stewart, W E., and Lightfoot, E. N. 1960. Transport Phenomena, Wiley,
New York, NY.
34. Patankar, S. V. 1980. Numerical Heat
Transfer and Fluid Flow, Hemisphere Publishing Corporation, New York, NY..
35. Voller, V R., and Prakash, C 1987. A
fixed grid numerical modelling methodology
for convection-diffusion mushy region phasechange problems. International Journal of Heat
and Mass Transfer 30: 1709-1720.
36. Brent, A. D., Voller, V. R., and Reid, K.
J. 1988. Enthalpy-porosity technique for modeling convection-diffusion phase change: Application to the melting of a pure metal. Numerical Heat Transfer 13: 297-318.
37. Zhang, W., Kim, C. H, and Deb-
Roy, T 2004. Heat and fluid flow in complex
joints during gas-metal arc welding. Part I: Numerical model of fillet welding. Journal of Applied Physics 95(9): 5210-5219.
38. Zhang, W., Kim, C. H, and DebRoy, T 2004. Heat and fluid flow in complex
joints during gas-metal arc welding. Part II: Application to Fillet Welding of Mild Steel. Journal
of Applied Physics 95(9): 5220-5229
39. Kumar, A, and DebRoy, T. 2003. Calculation of Three-Dimensional Electromagnetic
Force Field during Arc Welding. Journal of Applied Physics 94: 1261-1211.
40. Kou, S., and Sun, D. K. 1985. Fluid flow
and weld penetration in stationary arc welds.
Metalurgical Transactions A 16A: 203-213.
41. Kim, C. H, Zhang, W., and DebRoy, T
2003. Modeling of temperature field and solidified surface profile during gas metal arc fillet
welding. Journal of Physics D: Applied Physics
94:2661-2619.
42. De, A, and DebRoy, T 2004. Probing
unknown welding parameters from convective
heat transfer calculation and multivariable optimization. Journal of Applied Physics 37(1):
140-150.
43. De, A., and DebRoy, T 2004. A smart
model to estimate effective thermal conductivity and viscosity in weld pool. Journal of Applied
Physics 95(9): 5230-5240.
44. DebRoy, T, and Majumdar, A. K. 1981.
Predicting fluid flow in gas stirred systems. Journal of Metals 33(11): 42-47.
45. Launder, B. E., and Spalding, D. B.
1972. Lectures in Mathematical Models of Turbulence, Academic Press, London, UK.
46. Hong, K. 1996. Ph.D. dissertation. University of Waterloo.
47. Yang, Z., and DebRoy, T 1999. Modeling of macro- and microstructures of gas-metalarc welded HSLA-100 steel. Metallurgical
Transactions B 30B: 483-493.
48. He, X., Elmer, J. W, and DebRoy, T.
2005. Heat Transfer and Fluid Flow in Laser Microwelding. Journal of Applied Physics 91: article* 84909.
o
<
LU
(/)
LU
0C
O
LU
5
WELDING JOURNAL